Multiple Nonstoichiometric Phases with Discrete Composition Ranges in the CaAu5-CaAu4Bi-BiAu2 System. A Case Study of the Chemistry of Spinodal Decomposition
Qisheng Lin; John D. Corbett; Journal of the American Chemical Society 132 (2010) 5662–5671; doi:10.1021/ja100250d

data_4102303
_publ_contact_author_address
;359 Spedding Hall
Iowa State University
Ames, IA, 50010
;
_publ_contact_author_email       jdc@ameslab.gov
_publ_contact_author_name        'John D Corbett'
_publ_section_title
;
 Multiple Nonstoichiometric Phases with Discrete Composition Ranges in the
 CaAu5-CaAu4Bi-BiAu2 System. A Case Study of the Chemistry of Spinodal
 Decomposition
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              5662
_journal_page_last               5671
_journal_paper_doi               10.1021/ja100250d
_journal_volume                  132
_journal_year                    2010
_chemical_formula_moiety         'Au8, 63.46(Bi0.04), 32.54(Ca0.04'
_chemical_formula_sum            'Au8 Bi2.64 Ca1.36'
_chemical_formula_weight         2182.65
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           216
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   7.9505(2)
_cell_length_b                   7.9505(2)
_cell_length_c                   7.9505(2)
_cell_measurement_reflns_used    736
_cell_measurement_temperature    273(2)
_cell_measurement_theta_max      27.68
_cell_measurement_theta_min      4.44
_cell_volume                     502.55(2)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      273(2)
_diffrn_measured_fraction_theta_full 0.981
_diffrn_measured_fraction_theta_max 0.981
_diffrn_measurement_device_type  'Smart Apex CCD'
_diffrn_measurement_method       w/
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0562
_diffrn_reflns_av_sigmaI/netI    0.0348
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            736
_diffrn_reflns_theta_full        27.68
_diffrn_reflns_theta_max         27.68
_diffrn_reflns_theta_min         4.44
_exptl_absorpt_coefficient_mu    163.007
_exptl_absorpt_correction_T_max  0.056
_exptl_absorpt_correction_T_min  0.025
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            METALLIC
_exptl_crystal_density_diffrn    14.425
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       irregular
_exptl_crystal_F_000             1757
_exptl_crystal_size_max          0.023
_exptl_crystal_size_mid          0.019
_exptl_crystal_size_min          0.017
_refine_diff_density_max         1.511
_refine_diff_density_min         -2.241
_refine_diff_density_rms         0.436
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.0(2)
_refine_ls_extinction_coef       0.00063(8)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.163
_refine_ls_matrix_type           full
_refine_ls_number_parameters     9
_refine_ls_number_reflns         85
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.163
_refine_ls_R_factor_all          0.0238
_refine_ls_R_factor_gt           0.0234
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0177P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0457
_refine_ls_wR_factor_ref         0.0461
_reflns_number_gt                84
_reflns_number_total             85
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja100250d_si_002_5.cif
_cod_data_source_block           crystal_5
_cod_original_formula_sum        'Au8 Bi2.64 Ca1.36 '
_cod_database_code               4102303